compound and polyhedral oligomeric silsesquioxane reagents ... case of the airbus a350 and boeing...
Post on 22-Mar-2020
Embed Size (px)
Kopsidas, S., & Hamerton, I. (2016). Examining the thermal behaviour of novel aromatic polybenzoxazine blends containing an organophosphorous compound and polyhedral oligomeric silsesquioxane reagents. Polymer International, 65(9), 1015-1023. https://doi.org/10.1002/pi.5139
Peer reviewed version
Link to published version (if available): 10.1002/pi.5139
Link to publication record in Explore Bristol Research PDF-document
University of Bristol - Explore Bristol Research General rights
https://research-information.bris.ac.uk/en/persons/ian-hamerton(b3d6ab4a-54e4-41a8-8eaa-d03d2893891a).html https://research-information.bris.ac.uk/en/publications/examining-the-thermal-behaviour-of-novel-aromatic-polybenzoxazine-blends-containing-an-organophosphorous-compound-and-polyhedral-oligomeric-silsesquioxane-reagents(b5f783f0-662c-483d-bd61-4c109c79c5f8).html https://research-information.bris.ac.uk/en/publications/examining-the-thermal-behaviour-of-novel-aromatic-polybenzoxazine-blends-containing-an-organophosphorous-compound-and-polyhedral-oligomeric-silsesquioxane-reagents(b5f783f0-662c-483d-bd61-4c109c79c5f8).html https://research-information.bris.ac.uk/en/publications/examining-the-thermal-behaviour-of-novel-aromatic-polybenzoxazine-blends-containing-an-organophosphorous-compound-and-polyhedral-oligomeric-silsesquioxane-reagents(b5f783f0-662c-483d-bd61-4c109c79c5f8).html https://doi.org/10.1002/pi.5139 https://doi.org/10.1002/pi.5139 https://research-information.bris.ac.uk/en/publications/examining-the-thermal-behaviour-of-novel-aromatic-polybenzoxazine-blends-containing-an-organophosphorous-compound-and-polyhedral-oligomeric-silsesquioxane-reagents(b5f783f0-662c-483d-bd61-4c109c79c5f8).html https://research-information.bris.ac.uk/en/publications/examining-the-thermal-behaviour-of-novel-aromatic-polybenzoxazine-blends-containing-an-organophosphorous-compound-and-polyhedral-oligomeric-silsesquioxane-reagents(b5f783f0-662c-483d-bd61-4c109c79c5f8).html
Examining The Thermal Behaviour of Novel Aromatic Polybenzoxazines Blends Containing
Organophosphorus Compounds and POSS Reagents
Sotirios Kopsidasa and Ian Hamerton*b
aDepartment of Chemistry, Faculty of Engineering and Physical Sciences, University of Surrey,
Guildford, Surrey, GU2 7XH, U.K.
bThe Advanced Composites Centre for Innovation and Science, Department of Aerospace
Engineering, University of Bristol, Queen’s Building, University Walk, Bristol, BS8 1TR, U.K.
*To whom correspondence should be addressed.
Abstract: 2,2-Bis(3,4-dihydro-3-phenyl-2H-1,3-benzoxazine)propane (BA-a) is blended with
different commercial polyhedral oligomeric silsesquioxane (POSS) reagents and an
organophosphorous compound bis(4-hydroxyphenyl)phenylphosphine oxide (BPPO), at a range of
loadings (1 – 10 wt %). The influence of the additives on the onset and a rate of polymerisation of the
BA-a is examined using differential scanning calorimetry. An initial screen of blends containing various
additives (5 wt%) shows that a combination of aminoethylaminopropyl isobutyl POSS (AEAP) and
BPPO has the greatest effect on reactivity with a reduction in reaction onset of some 65 K and an
increase in Tg of 18 K when compared with the BA-a homopolymer. The activation energy for the
polymerization of BA-a containing 5 wt% AEAP was determined to be 84-88 kJ/mol (using
Kissinger and Ozawa kinetic models), with a first order rate constant of 1.9 x 108 s-1. The thermal
stability of the cured blends containing 5 wt% flame retardant were examined using
thermogravimetric analysis (TGA) and both onset of degradation and char yield are increased by 15
K and 5 % respectively when compared with the BA-a homopolymer.
Keywords: Polybenzoxazines, flame retardants, POSS reagents, organophosphorous compounds,
polymerisation kinetics, thermal stability, nanocomposites.
Polymers and their composites are being applied increasingly in the aerospace industry in recent
years , more recently composites have been used in commercial airliners, most notably in the
case of the Airbus A350 and Boeing 787 which comprise up to 50 % composite by volume [2,3].
Composites are now being applied in the primary structure of aircraft so their integrity is very
important, developing methods to improve toughness of neat resins and trying to understand how
the toughening agent works is the first step in developing robust composites. Polybenzoxazines
(PBZs) show promising thermal and mechanical performance for these applications, but
improvements in toughness are required before this can be a reality. The potential for the use of
oligomers based on engineering thermoplastics have been examined for some years as modifiers in
aerospace composite matrices [4,5], due to their inherent toughness and the ability to blend them
more easily than high molecular weight species without incurring the penalty of high melt viscosity.
The high aromatic content and potential to produce high yields of char during combustion make
PBZs particularly attractive in an environment in which the polymer industry has moved away from
the extensive use that was made of halogenated polymers or halogenated additives .
Another considerable drawback of BZ monomers is that they are typically slow to react, requiring
curing temperatures in the range of 200 C [7,8]. High curing temperatures are a major limitation
for the adoption of PBZs in advanced industrial applications, when compared to other competitor
resins; for instance, epoxies may be cured at comparatively modest temperatures (60 C and 120
C), yet still achieve relatively high values of glass transition temperature (dry Tg = 150 C).
Compounds containing an active hydrogen atom, such as carboxylic acids and phenols have been
widely established as effective catalysts for the ring-opening polymerisation of BZ monomers ,
which as already mentioned proceeds via a cationic mechanism. However, from the viewpoint of
practical applications, the use of strong catalysts may severely compromise the shelf life of one-pot
formulations [9, 10]. Other compounds that have been investigated as initiators include Lewis acids
, bi-functional catalysts , phosphonic and sulfonic acids as well as basic compounds such as
imidazoles and amines , and the latter are examined in this work.
Polyhedral oligomeric silsesquioxane (POSS) reagents have attracted considerable interest in the
area of polymer nanocomposites, since they demonstrate excellent properties as nano-phase
additives or nano-scale modifiers , including high thermal stability and good mechanical
properties [15,16,17]. Thus, they are an active and important part of the system. POSS reagents are
inorganic ceramic-like nanocages that comprise a silicon-oxygen framework. A typical POSS
molecule possesses a rigid cubic structure, represented by the formula R8Si8O12, where the central
inorganic core (Si8O12) is functionalised with organic moieties (R) at up to eight corners ,
although more typically mono- or difunctional species are used. This class of hybrid materials has
the ability to improve the mechanical properties of polymer nanocomposites, as the incorporation of
small amounts into the polymer matrix can have a positive impact on various features, such as the
modulus, Tg and fracture toughness. Ormasil nanoparticles can lead to changes in toughness, but
also mechanism . In addition, POSS fillers have been proven to enhance significantly the
thermal stability of polymer blends, a property that arises from the thermally stable inorganic Si-O
The preparation of PBZs incorporating functionalised POSS reagents dates from 2004  and, in
common with other families of high performance polymers, there has been a steady growth in
interest in the use of both mono- and poly-functional POSS reagents with PBZs with several
research groups concentrating on their exploration. Common approaches have utilised
appropriately functionalised POSS reagents to effect co-reaction with the oxazine ring, thus vinyl
groups [20,21] and glycidyl ethers . Alongside the more numerous studies to examine the
effects of blending POSS with PBZ and its blends or copolymers such as bisoxazolines  or
epoxies , is the use of benzoxazines as pendant groups within more flexible fluoropolymer films
. Less common is the use of more sophisticated synthetic methodologies such as the use of
click chemistry  to introduce benzoxazine functionality into the POSS reagent, but a model
POSS reagent with mixed functionality, allowing the potential for the formation of an A-B
copolymer has been reported [27